A facile approach to synthesize SiO2 · Re2O3 (Re = Y, Eu, La, Sm, Tb, Pr) hollow sphere and its application in drug release
© Li et al.; licensee Springer. 2013
Received: 21 June 2013
Accepted: 27 September 2013
Published: 21 October 2013
Multifunctional SiO2 · Re2O3 (Re = Y, Eu, La, Sm, Tb, Pr) hollow spheres (HSs) have been fabricated using an acidic Re3+ ion solution. Under ultraviolet radiation, functional HSs emit different colors of light according to the different rare-earth ions embedded into the shell of SiO2 hollow spheres. The as-prepared hollow capsules were characterized by X-ray diffraction, transmission electron microscopy, high-resolution transmission electron microscopy, Brunauer-Emmett-Teller method, scanning electron microscopy, and energy-dispersive spectrometry. Drug loading and release experiments have been carried out using SiO2 · Eu2O3 HSs that acted as drug carriers. The results demonstrate that the multifunctional HSs exhibit a high storage capacity and the ability of retaining drug stability and activity, which indicates that the as-synthesized fluorescent hollow capsules are a potential candidate as drug delivery materials.
KeywordsSiO2 · Re2O3 Hollow spheres (HSs) Fluorescence
Recently, much attention have been focused on the research of hollow SiO2 spheres (HSSs) because of their excellent properties such as thermal stability, large surface areas, low density, low toxicity, and good compatibilities with other materials [1–15]. So, HSSs have attracted intense interest and have been widely applied in a variety of fields, such as catalysis, sensors, chromatography, dyes, inks, photonic crystals, cells, waste removal, shield for enzymes or proteins, delivery vehicle of drugs, and large biomolecular release [16–28]. In general, three approaches are employed to prepare HSSs: template methods [6, 29–31], self-assembly technique, and microemulsions [32, 33]. HSSs [34–36] have been fabricated with the soft template and hard template methods, which involve complicated procedures such as shell formation and core removal. The template-free method has attracted much attention due to its simple and economical characteristic [27, 28]. In 2008, Zhang et al.  developed a self-template method to convert solid silica into hollow spheres (HSs). In the process, silica is dissolved into NaBH4 solution and silicate species deposited on the surface of the silica colloid. The shell formed over the silicate species via Ostwald ripening results in HSSs. An alkalescent environment is an inevitable synthesis condition that is reported in nearly all papers [37–50]; the only exception is that of Chen et al. who used HF as an etching agent . In 2011, Wang’s group reported firstly the synthesis of HSSs in generic acidic media . Unfortunately, the published work was based on the study of only two factors: pH value and Na+ ion, which influence the formation process of HSSs.
Herein, we report a one-step self-driven process to synthesize multifunctional HSSs under an acidic condition with rare-earth ion assistance. Compared with Wang’s report, the synthetic approach of HSSs is simpler. Being synthesized with the assistance of rare-earth ions, the as-prepared HSSs can emit bright fluorescence under ultraviolet radiation, which is convenient to be detected in real time if it is used in biological applications. Typical drug loading and release experiments are carried out using our prepared multifunctional HSSs, SiO2 · Eu2O3 HSs.
All chemicals were of analytical grade and purchased from Jinan Camolai Trading Company (Jinan, China), which were used as received without further purification: tetraethyl orthosilicate (TEOS, 98%), ammonium hydroxide solution (NH3 · H2O, approximately 25% in water), nitric acid (HNO3, 65%), Re2O3, and ethanol (C2H5OH). Rare-earth nitrate solutions [Re(NO3)3 (Re = Y, Eu, La, Sm, Tb, Pr)] with a concentration of 0.04 to 0.08 mol/L were prepared by ourselves.
Synthesis of monodisperse silica spheres
Synthesis of SiO2 · Re2O3 hollow spheres
In a typical synthesis, silica spheres (0.06 g) were added to 20 mL Re(NO3)3 (0.06 mol/L) and stirred for 30 min. The pH of the solution is 4.5 (adjusted with dilute nitric acid). The mixture was transferred into a Teflon-lined stainless autoclave (capacity 25 mL) and heated at 250°C for 12 h. After the products naturally cooled down to room temperature, they were washed with deionized water and separated by centrifugation (4,000 rpm) for three times and then dried at 60°C for 4 h in the air.
Drug storage and release
SiO2 · Eu2O3 HSs (1 g) were added into a 50-mL hexane solution containing 40 mg/mL ibuprofen (IBU). The mixture was sealed and stirred for 24 h. Then the sample was separated by centrifugation and dried at 60°C in the air. The filter was characterized by UV-visible (UV–vis; 264 nm) spectroscopy.
The dry SiO2 · Eu2O3 loaded with IBU (0.1 g) was immersed into 50 mL of simulated body fluid (SBF; pH = 7.4) at 37°C and stirred at the rate of 100 rpm. Three milliliters from the top of the solution was used for release measurement at different intervals, and then 3 mL of fresh SBF is added into the solution to keep the volume unchanged.
Characterization and instruments
The samples were characterized by X-ray diffraction (XRD) with a Philips X’Pert Super diffractometer (Amsterdam, The Netherlands) with graphite-monochromatized Cu Kα radiation (λ = 1.54178 Å) in the 2θ range of 1.5° to 10° and 10° to 80°.
The transmission electron microscopy (TEM) images and electron diffraction (ED) patterns were obtained using a Hitachi 800 transmission electron microscope (Chiyoda-ku, Japan) with an accelerating voltage of 200 kV.
The high-resolution transmission electron microscopy (HRTEM) images were obtained using JEOL-2010 (Akishima-shi, Japan).
The UV–vis absorption spectra of the samples were measured using a UV-1800 ultraviolet–visible spectrophotometer (Shanghai Meipuda Instrument Co., Ltd., Shanghai, China).
The samples used for characterization were ultrasonically dispersed in absolute ethanol for 30 min before the TEM and HRTEM tests.
Results and discussion
Characterization of SiO2 · Eu2O3 HSs
Influencing factors of the synthetic process of SiO2 · Re2O3 (Re = Y, Eu, La, Sm, Tb, Pr) hollow structures
The experiments showed that the pH value of the solution, reaction temperature and time, and different rare-earth ions and concentrations played an outstanding role in the synthesis of SiO2 · Re2O3 hollow structures, which are discussed in detail as follows.
Effect of the pH value of the solution
The pH value of the solution was adjusted with dilute nitric acid. The studied pH range was from 7 to 3 under the following reaction conditions: Re3+ = 0.06 mol/L and T = 250°C. Hollow-structure particles could be obtained under the range of 4 ≤ pH < 5.5, and the optimum pH value was 4.5. No hollow structure products appeared when 6 ≤ pH ≤ 8. No HSSs appeared when 2 < pH < 3. Normally, a few HSSs could have emerged in the product at the conditions of 3 < pH < 4.0 or 5 < pH < 6 if the reaction time was more than 10 h. The detailed results are shown in Additional file 1: Table S1 and Figure S3. It is known that SiO2 is an amphoteric oxide which can dissolve into an acidic or basic solvent. The experiments showed that a weak acid solution was in favor of hollow structure formation. The experiments also revealed that the experimental results were unaffected when using other acids such as HCl or H2SO4 to adjust the pH value of the solution.
Effect of reaction temperature
The temperature of the hydrothermal reaction affected greatly not only the reaction (going or not) but also the reaction rate (slow or fast). Additional file 1: Figure S1 shows the TEM images of the as-prepared samples at different reaction temperatures. No hollow-structure products appeared if the temperature T < 230°C in our experiments. The morphology and size of nanocrystals became difficult to control when the temperature was up to 260°C or higher because the higher the temperature was, the faster the reaction rate was. When T = 255°C, the quality of the obtained SiO2 · Re2O3 HSs was always poor. The experiments verify that the moderate temperature was 250°C.
Effect of Re3+ ion and its concentration
It was reported that Na2SO4 and NaCl were advantageous to HSS formation  and the work matter was Na+ cation, which was in line with our experimental data. Hereby, we investigated the synthesis of HSSs under different rare-earth ions and bivalent cations.
In order to get uniform hollow structures, the optimal concentration of the rare-earth ions was usually kept in the range of 0.04 to 0.08 mol/L. The experimental data and TEM images are depicted in Additional file 1: Table S1 and Figure S2. The concentration less than 0.03 mol/L resulted in poor quality in production, and the concentration greater than 0.08 mol/L always led to products with not all having a hollow structure. The experiments showed that the lower or higher concentration of Re3+ ions was not good for HSS formation and 0.06 mol/L was the optimal concentration.
Although the SiO2 · Re2O3 HSs were obtained based on the rare-earth ion assistance strategy, their quality was quite different under assistance of different kinds of rare-earth ions. By keeping other reaction conditions unchanged such as the pH value of the solution, reaction time, and reaction temperature, the influence of different Re3+ ions (Re = Y, Eu, La, Sm, Tb, Pr) on the structure of the as-prepared products was investigated (see Additional file 1: Table S2 and Figure S4). Additional file 1: Figure S4 clearly shows that the influence sequence of Re3+ was as follows: Eu3 + ≈ Sm3 + > Y3 + > Pr3 + ≈ La3 + > Tb3 +. Nearly all of the as-prepared samples were hollow spheres with good quality under the effect of Eu3+ and Sm3+ existence, and the experiments showed good reproducibility and satisfactory results. With Y3+, Pr3+, and La3+ ions included, all of the products always formed a mixture of HSSs and core/shell structure. Furthermore, all of the samples can be formed into a hollow sphere if the reaction time is prolonged, but the yield of HSSs was lower. Only a small amount of HSs could be obtained with Tb3+ existence. The experiments indicated that changing the reaction time did not work.
We compared the synthesis approach under the same reaction conditions using Mg2+, Ca2+, Mn2+, Zn2+, and Cu2+ instead of Re3+ ions. The results showed that SiO2 · HSs could barely be obtained at the above situations, which indicated that rare-earth ion was an indispensable factor in hollow structure formation.
Experimental data showed that the rare-earth ions were advantageous to HSS formation; however, further study is needed to understand why the effect of different Re3+ ions on the formation of HSSs has a different role.
Effect of reaction time
From the above, our synthesis procedure of HSSs is very simple and effective compared with those previously reported.
Formation mechanism of SiO2 · Re2O3 HSs
The experiments showed that the diameter of SiO2 · Re2O3 HSs was almost the same as that of the template, which indicated that the size of SiO2 · Re2O3 HSs was determined by the SiO2 solid spheres. Therefore, we can control the size of SiO2 · Re2O3 HSs by controlling the diameter of SiO2 solid spheres.
Drug delivery and release
Considering that HSs have numerous mesoporous structures on the surface, they can act as drug loading capsules. IBU, a typical anti-inflammatory drug, is a good example used for drug loading experiments [49, 53]. Herein, IBU was used to study the drug delivery and release behavior of nanostructured HSs.
The SiO2 · Re2O3 HSs were 1 g after loading IBU (see the ‘Methods’ section), and the IBU storage in nanostructured SiO2 · Re2O3 HSs reached 287.8 mg/g, which means that the as-prepared SiO2 · Re2O3 HSs have a high loading capacity.
where R is the total release rate, C i is the IBU concentration in SBF at time i, i is the time of the IBU medium solution taking out from the SBF, and m represents the total mass of the IBU in the HSs.
Figure 7A shows the release behavior of the IBU-loaded SiO2 · Eu2O3 HSs in SBF. Compared with the pure IBU disk release in SBF, the release rate of the IBU-loaded SiO2 · Eu2O3 HSs lasted long. The drug release rate was very fast within 12 h, which showed a nearly linear relationship between drug release rate and release time at the first 12 h. Then the drug release process was very slow and finished after 60 h. The results indicated that the sustained release behavior of the drug carrier was in favor of a durative drug effect.
In order to investigate the properties of the loaded drug, the UV–vis absorption spectra of the IBU hexane solution before and after IBU loading in SiO2 · Eu2O3 HSs were measured. The results are shown in Figure 7B. Curves a, b, and c were the IBU hexane solution before drug loading, the SBF solution after the release of IBU-loaded SiO2 · Eu2O3 HSs for 4 h, and the SBF solution after the release of IBU-loaded SiO2 · Eu2O3 HSs for 70 h, respectively. It was noticed that the shape of the absorption curves was essentially the same, which demonstrated that the property of IBU was not changed in the loading and release processes.
We noticed that the samples still emitted fluorescence after the experiments of drug delivery and release, which indicated that the leftover via the loading and release processes can be tracked and detected.
We have reported an approach of the synthesis of functional SiO2 · Re2O3 HSs using silica spheres, rare-earth ions, and an acidic environment. The size of synthesized hollow capsules can be modulated by controlling the diameter of the silica template. The facile and economical synthesis protocol is valuable and convenient for wide use. Acting as drug-loaded capsules, the SiO2 · Re2O3 HSs demonstrated much excellent properties of high payloads, retained drug activity and stability, and slow drug release rate. Furthermore, real-time detection may be carried out during drug delivery and release with SiO2 · Re2O3 HSs by measuring their fluorescence.
The authors express their thanks to Associate Prof. Rusen Yang (University of Minnesota) for the language polishing.
- Van Bommel KJC, Jung JH, Shinkai S: Poly(L-lysine) aggregates as templates for the formation of hollow silica spheres. Adv Mater 2001, 3(19):1472–1476.View ArticleGoogle Scholar
- Fan WG, Gao LJ: Synthesis of silica hollow spheres assisted by ultrasound. J Colloid Interf Sci 2006, 297(1):157–160. 10.1016/j.jcis.2005.10.021View ArticleGoogle Scholar
- Yeh YQ, Chen BC, Lin HP, Tang CY: Synthesis of hollow silica spheres with mesostructured shell using cationic-anionic-neutral block copolymer ternary surfactants. Langmuir 2006, 22(1):6–9. 10.1021/la052129yView ArticleGoogle Scholar
- Zhu GS, Qiu SL, Terasaki O, Wei YJ: Polystyrene bead-assisted self-assembly of microstructured silica hollow spheres in highly alkaline media. Am Chem Soc 2001, 123(31):7723–7724. 10.1021/ja0158758View ArticleGoogle Scholar
- Caruso F: Nanoengineering of particle surfaces. Adv Mater 2001, 13: 11–22. 10.1002/1521-4095(200101)13:1<11::AID-ADMA11>3.0.CO;2-NView ArticleGoogle Scholar
- Tissot I, Reymond JP, Lefebvre F, Bourgeat-Lami E: SiOH-functionalized polystyrene latexes. A step toward the synthesis of hollow silica nanoparticles. Chem Mater 2002, 14: 1325–1331. 10.1021/cm0112441View ArticleGoogle Scholar
- Liu SQ, Lu LC, Sui XY, Vera M, Pegie C, Etienne FV: Fast fabrication of hollow silica spheres with thermally stable nanoporous shells. Microporous Mesoporous Mater 2007, 98: 41–46. 10.1016/j.micromeso.2006.08.014View ArticleGoogle Scholar
- Chen YW, Kang ET, Neoh KG, Grener A: Preparation of hollow silica nanospheres by surface-initiated atom transfer radical polymerization on polymer latex templates. Adv Funct Mater 2005, 15(1):113–117. 10.1002/adfm.200400179View ArticleGoogle Scholar
- Darbandi M, Thomann R, Nann T: Silica coated nanocomposites. Chem Mater 2007, 19(7):1700–1703. 10.1021/cm062803cView ArticleGoogle Scholar
- Deng ZW, Chen M, Zhou S, You B, Wu LM: A novel method for the fabrication of monodisperse hollow silica spheres. Langmuir 2006, 22: 6403–6407. 10.1021/la060944nView ArticleGoogle Scholar
- Chen M, Wu L, Zhou S, You B: A method for the fabrication of monodisperse hollow silica spheres. Adv Mater 2006, 18: 801–805. 10.1002/adma.200501528View ArticleGoogle Scholar
- Tsai MS, Li MJJ: A novel process to prepare a hollow silica sphere via chitosan-polyacrylic acid (CS-PAA) template. Non-Cryst Solids 2006, 352(26–27):2829–2833.View ArticleGoogle Scholar
- Botterhuis NE, Sun QY, Magusin PCMM, Van Santen RA, Sommerdijk NA: Hollow silica spheres with an ordered pore structure and their application in controlled release studies. Chem-Eur J 2006, 12(5):1448–1456. 10.1002/chem.200500588View ArticleGoogle Scholar
- Han YS, Jeong GY, Lee SY, Kim HKJ: Hematite template route to hollow-type silica spheres. Solid State Chem 2007, 180: 2978–2985. 10.1016/j.jssc.2007.08.016View ArticleGoogle Scholar
- Wan Y, Yu SHJ: Polyelectrolyte controlled large-scale synthesis of hollow silica spheres with tunable sizes and wall thicknesses. Phys Chem C 2008, 112(10):3641–3647. 10.1021/jp710990bView ArticleGoogle Scholar
- Chen Y, Chen HR, Guo LM, He QJ, Chen F, Zhou J, Feng JW, Shi JL: Hollow/rattle-type mesoporous nanostructures by a structural difference-based selective etching strategy. ACS Nano 2010, 4: 529–539. 10.1021/nn901398jView ArticleGoogle Scholar
- Lou XW, Archer LA, Yang ZC: Hollow micro-/nanostructures: synthesis and applications. Adv Mater 2008, 20: 3987–4019. 10.1002/adma.200800854View ArticleGoogle Scholar
- Ding SJ, Chen JS, Qi G, Duan X, Wang Z, Giannelis EP, Archer LA, Lou XWJ: Formation of SnO2 hollow spheres inside silica nanoreactors. Am Chem Soc 2011, 133: 21–23. 10.1021/ja108720wView ArticleGoogle Scholar
- Zhang Q, Ge JP, Goebl J, Hu YX, Lu ZD, Yin YD: Rattle-type silica colloidal particles prepared by a surface-protected etching process. Nano Res 2009, 2: 583–591. 10.1007/s12274-009-9060-5View ArticleGoogle Scholar
- Tan LF, Chen D, Liu HY, Tang FQ: A silica nanorattle with a mesoporous shell: an ideal nanoreactor for the preparation of tunable gold cores. Adv Mater 2010, 22: 4885–4889. 10.1002/adma.201002277View ArticleGoogle Scholar
- Sanles-Sobrido M, Exner W, Rodríguez-Lorenzo L, Rodríguez-Gonzalez B, Correa-Duarte MA, Alvarez-Puebla RA, Liz-Marzan LM: Design of SERS-encoded, submicron, hollow particles through confined growth of encapsulated metal nanoparticles. J Am Chem Soc 2009, 131: 2699–2705. 10.1021/ja8088444View ArticleGoogle Scholar
- Li LL, Tang FQ, Liu HY, Liu TL, Hao NJ, Chen D, Teng X, He JQ: In vivo delivery of silica nanorattle encapsulated docetaxel for liver cancer therapy with low toxicity and high efficacy. ACS Nano 2010, 4: 6874–6882. 10.1021/nn100918aView ArticleGoogle Scholar
- Ren N, Wang B, Yang YH, Zhang YH, Yang WL, Yue YH, Gao Z, Tang Y: General method for the fabrication of hollow microcapsules with adjustable shell compositions. Chem Mater 2005, 17: 2582–2587. 10.1021/cm0502828View ArticleGoogle Scholar
- Yamada Y, Mizutani M, Nakamura T, Yano K: Mesoporous microcapsules with decorated inner surface: fabrication and photocatalytic activity. Chem Mater 2010, 22: 1695–1703. 10.1021/cm9031072View ArticleGoogle Scholar
- Zhang Q, Zhang TR, Ge JP, Yin YD: Permeable silica shell through surface-protected etching. Nano Lett 2008, 8: 2867–2871. 10.1021/nl8016187View ArticleGoogle Scholar
- Cao S, Fang L, Zhao Z, Ge Y, Piletsky S, Anthony P, Turner F: Hierachically structured hollow silica spheres for high efficiency immobilization of enzymes. Adv Funct Mater 2013, 23(17):2162–2167. 10.1002/adfm.201201793View ArticleGoogle Scholar
- Zhang TR, Ge JP, Hu YX, Zhang Q, Aloni S, Yin YD: Formation of hollow silica colloids through a spontaneous dissolution–regrowth process. Angew Chem Int Ed 2008, 47: 5806–5811. 10.1002/anie.200800927View ArticleGoogle Scholar
- Zhang TR, Zhang Q, Ge JP, Goebl J, Sun MW, Yan YS, Liu YS, Chang CL, Guo JH, Yin YDJ: A self-templated route to hollow silica microspheres. Phys Chem C 2009, 113: 3168–3175. 10.1021/jp810360aView ArticleGoogle Scholar
- Yang ZZ, Niu ZW, Lu YF, Hu Z, Han Charles C: Templated synthesis of inorganic hollow spheres with a tunable cavity size onto core–shell gel particles. Angew Chem Int Ed 2003, 115: 1987–1989. 10.1002/ange.200250443View ArticleGoogle Scholar
- Zhong Z, Yin Y, Gates B, Xia Y: Preparation of mesoscale hollow spheres of TiO2 and SnO2 by templating against crystalline arrays of polystyrene beads. Adv Mater 2000, 12: 206–209. 10.1002/(SICI)1521-4095(200002)12:3<206::AID-ADMA206>3.0.CO;2-5View ArticleGoogle Scholar
- Wang X, Miao X-R, Li Z-M, Deng W-L: Fabrication of microporous hollow silica spheres templated by NP-10 micelles without calcinations. Appl Surf Sci 2011, 257: 2481–2488. 10.1016/j.apsusc.2010.10.005View ArticleGoogle Scholar
- Okubo M, Ito A, Kanenobu T: Production of submicron-sized multihollow polymer particles by alkali/cooling method. Colloid Polym Sci 1996, 274: 801–804. 10.1007/BF00654677View ArticleGoogle Scholar
- Li W, Sha X, Dong W, Wang Z: Synthesis of stable hollow silica microspheres with mesoporous shell in nonionic W/O emulsion. Chem Commun 2002, 20: 2434–2435.View ArticleGoogle Scholar
- Zi-Wei D, Min C, Shu-Xue Z, Bo Y, Li-Min W: A facile approach for the fabrication of monodisperse hollow silica spheres. Chem J Chin U 2006, 27(10):1795–1799.Google Scholar
- Wu XF, Tian YJ, Cui YB, Wei LQ, Wang Q, Chen YF: Raspberry-like silica hollow spheres: hierarchical structures by dual latex-surfactant templating route. J Phys Chem C 2007, 111: 9704–9708. 10.1021/jp070811qView ArticleGoogle Scholar
- Lou X, Schumacher T, Yang H, Ding A: Synthesis and characterisation of silica–polymer hybrid core–shell and hollow spheres for drug delivery. J Control Release 2011, 152: e1-e132.View ArticleGoogle Scholar
- Stober W, Fink A, Bohn EJ: Controlled growth of monodisperse silica spheres in the micron size range. Colloid Interface Sci 1968, 26: 62–69. 10.1016/0021-9797(68)90272-5View ArticleGoogle Scholar
- Wang W, Gu BH, Liang LY, Hamilton WJ: Fabrication of two- and three-dimensional silica nanocolloidal particle arrays. Phys Chem B 2003, 107: 3400–3404. 10.1021/jp0221800View ArticleGoogle Scholar
- Lu LH, Capek R, Kornowski A, Gaponik N, Eychmuller A: Selective fabrication of ordered bimetallic nanostructures with hierarchical porosity. Angew Chem Int Ed 2005, 44: 5997–6001. 10.1002/anie.200501471View ArticleGoogle Scholar
- Blasse G, Grabmaier BC: How does a luminescent material absorb its excitation energy? Luminescence Materials. New York: Springer; 1994:22.Google Scholar
- Shionoya S, Yen WM: Principal phosphor materials and their optical properties. Phosphor Handbook. Boca Raton: CRC Press; 1999:190.Google Scholar
- Mho S-I, Wright JC: Site selective spectroscopy of defect chemistry in CdF2:Eu. J Chem Phys 1982, 77: 1183. 10.1063/1.443984View ArticleGoogle Scholar
- Judd BR: Optical absorption intensities of rare-earth ions. Phys Rev 1962, 127: 750. 10.1103/PhysRev.127.750View ArticleGoogle Scholar
- Ofelt GS: Intensities of crystal spectra of rare-earth ions. J Chem Phys 1962, 37: 511. 10.1063/1.1701366View ArticleGoogle Scholar
- Zeng HC: Ostwald ripening: a synthetic approach for hollow nanomaterials. Curr Nanosci 2007, 3: 177–181. 10.2174/157341307780619279View ArticleGoogle Scholar
- Zhang H, Zhao Y, Daniel L, Akins J: Synthesis and new structure shaping mechanism of silica particles formed at high pH. J Solid State Chem 2012, 194: 277–281.View ArticleGoogle Scholar
- Zhu H, Yang D, Zhu L, Li D, Chen P, Yu G: Hydrothermal synthesis and photoluminescence properties of La2−xEu x Sn2O7 ( x = 0–2.0) nanocrystals. J Am Ceram Soc 2007, 90: 3095. 10.1111/j.1551-2916.2007.01851.xView ArticleGoogle Scholar
- Yuan J, Wang Z: A facile method of synthesis of asymmetric hollow silica spheres. J Colloid Interface Sci 2011, 362: 15–20. 10.1016/j.jcis.2011.06.022View ArticleGoogle Scholar
- Ma M-Y, Zhu Y-J, Li L, Cao S-W: Nanostructured porous hollow ellipsoidal capsules of hydroxyapatite and calcium silicate: preparation and application in drug delivery. J Mater Chem 2008, 18: 2722–2727. 10.1039/b800389kView ArticleGoogle Scholar
- Abbas A, Borujeni AA, Najafi M, Hajian A: Synthesis and characterization of supported silica nano hollow spheres with CdS quantum dots. J Mol Liq 2012, 174: 124–128.View ArticleGoogle Scholar
- Chen D, Li LL, Tang FQ, Qi S: Facile and scalable synthesis of tailored silica “nanorattle” structures. Adv Mater 2009, 21: 3804–3807. 10.1002/adma.200900599View ArticleGoogle Scholar
- Yu Q, Wang P, Hu S, Hui J, Zhuang J, Wang X: Hydrothermal synthesis of hollow silica spheres under acidic conditions. Langmuir 2011, 27: 7185–7191. 10.1021/la200719gView ArticleGoogle Scholar
- Zhu Y, Fang Y, Borchardt L, Kaskel S: PEGylated hollow mesoporous silica nanoparticles as potential drug delivery. Micropor Mesopor Mat 2011, 141: 199–206. 10.1016/j.micromeso.2010.11.013View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an open access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.